the plane strain young’s modulus in cubic materials .the plane strain young’s modulus in cubic
Post on 27-May-2019
Embed Size (px)
J Elast (2017) 128:147173DOI 10.1007/s10659-017-9621-x
The Plane Strain Youngs Modulus in Cubic Materials
Kevin M. Knowles1
Received: 19 August 2016 / Published online: 31 January 2017 The Author(s) 2017. This article is published with open access at Springerlink.com
Abstract The orientation dependence of the plane strain Youngs modulus, E, of cubicmaterials has been analysed as a function of the direction along which a uniaxial stress isapplied to a single crystal and the perpendicular direction in the single crystal along whichthe strain is constrained to be zero. The locus of E in the plane perpendicular to the axis ofuniaxial stress is shown to be a circle when this stress is applied along 111. For materialswith anisotropy ratios A > 1, global minima in E occur when the stress is applied along001 and when the strain along one of the two perpendicular 100 directions is set tozero. Identical global maxima in E are found when the stress is applied along two differentfamilies of uuw directions and the direction of zero strain is along either a perpendicular110 or ww2u direction. For materials with A < 1, the global maxima in E occur whenthe stress is applied along 001 and when the strain along one of the two perpendicular100 directions is set to zero, and identical global minima are found when the stress isapplied along two different families of uuw directions and the direction of zero strain isalong either a perpendicular 110 or ww2u direction.Keywords Anisotropy Cubic materials Elasticity Plane strain Tensor algebraMathematics Subject Classification 74E10 74E15 74B05
There are a number of physical situations in which it is convenient to invoke the concept ofplane strain in elasticity problems. In isotropic elasticity, plane strain problems are definedin terms of plane strain displacements u1 and u2 within an x1x2 plane being functions onlyof the Cartesian coordinates x1 and x2, with the deformation u3 parallel to the direction x3perpendicular to both x1 and x2 being set to zero . Examples of such physical situations
B K.M. Knowleskmk10@cam.ac.uk
1 Department of Materials Science and Metallurgy, University of Cambridge, 27 Charles BabbageRoad, Cambridge, CB3 0FS, UK
148 K.M. Knowles
given by Timoshenko and Goodier include tunnels and retaining walls with lateral pressure,as in the walls of dams . Other examples where plane strain conditions are invoked arein elastic contact problems where each solid can be considered to be an elastic half-space, the analysis of the bending of relatively wide beams, in which the transverse bending isrestricted within the central portion of the beam [3, 4] and the plane strain elastic compres-sion of polycrystalline metals prior to plastic deformation, such as in cold rolling or forgingoperations. If, in isotropic elasticity, x1, x2 and x3 define the axes of the principal stresses11, 22 and 33 in such situations, and if furthermore 22 = 0, then the ratio 11/11 of theapplied stress to the induced elastic strain parallel to the applied stress is simply E/(1 2),where E is Youngs modulus and is Poissons ratio . This ratio is often described as theplane strain Youngs modulus .
For an anisotropic material, Ting  shows that the situation is more complex than forisotropic materials, so that u3 and the shear strains 13 and 23 do not have to be zero. How-ever, it is still the case that the tensile strain 33 is zero for a condition of a generalised planestrain deformation in an anisotropic material. Therefore, as Hopcroft et al. recognise in theirdiscussion of the plane strain Youngs modulus for single crystal silicon in connection withthe small deflections of short, relatively wide beams , the plane strain Youngs modulusfor a situation where 22 = 0 is a function of the orientation of the direction x1 along whichthe stress is applied in the x1x2 plane and the perpendicular direction x3 along which 33is zero. Hence, the plane strain Youngs modulus for silicon is orientation dependent, andtherefore potentially an important consideration in the design of micromechanical systemsusing silicon.
Interestingly, while the orientation dependence of the Youngs modulus of anisotropiccrystalline materials is well known  and the orientation dependence and extrema of Pois-sons ratio in particular as function of orientation has been a subject of recent interest [9,10], not least because of the concept of auxeticity , the specifics of the orientation de-pendence of the plane strain Youngs modulus have not been addressed, even in what mightbe expected to be the relatively straightforward case of cubic materials such as silicon. It isthe purpose of this paper to consider this orientation dependence and to identify extrema inthe plane strain Youngs modulus for cubic crystals as a function of the three independentelastic constants c11, c12 and c44 in contracted Voigt notation (see the Appendix), which arethemselves subject to the constraints that c44 > 0, c11 > |c12| and c11 + 2c12 > 0, follow-ing from the condition that the strain energy of a crystal must be positive [7, 8]. As Nyenotes , the three unique elastic compliance constants s11, s12 and s44 for cubic crystals aresubject to identical constraints.
The paper is organised as follows. A statement of the problem of determining the planestrain Youngs modulus for a plane of a general anisotropic material subject to a specificdirection within that plane not being strained is given in Sect. 2 before attention is focused onthe general form of the formula relevant to cubic materials. The application of this formulato directions along which a stress is applied lying in a standard stereographic triangle, ordirections related to these by symmetry, is considered in detail in Sect. 3. As a result ofthis, extrema are identified, both within planes perpendicular to the direction of appliedstress, and globally for combinations of directions of applied stress and specific directionsperpendicular to this direction not being strained as a function of c11, c12 and c44. Practicalconsequences of the results established in Sect. 3 are considered in Sect. 4.
The Plane Strain Youngs Modulus in Cubic Materials 149
2 General Tensor Transformation Relations for Plane Strain YoungsModulus
Under the assumption that elastic conditions pertain, the symmetric stress and strain tensors,ij and kl respectively, are related to one another through the equations
ij = Cijklkl and ij = Sijklkl, (1)in which Cijkl is the stiffness tensor and Sijkl is the compliance tensor, both tensors of thefourth rank, and where i, j , k and l take all values between 1 and 3 [5, 7, 8, 12, 13]. Foran arbitrary rotation of axes from one axis system to another, fourth rank tensors, Tijkl ,transform as
T ijkl = aimajnakpalqTmnpq, (2)for i, j , k, l, m, n, p and q all taking values from 1 to 3, where the aim are direction cosinesspecifying the angle between the ith axis of the new axis system and the mth axis of theold axis system. Both the old axis system and the new axis system in this formalismare defined by orthonormal axis systems. For materials with relatively high symmetry, oldaxis systems are straightforward to define with respect to the crystal axes, whereas this isnot the case with monoclinic or triclinic symmetry .
Defining axes 1, 2 and 3 as the axes in the new axis system parallel to the axes ofprincipal stress, with the primes to denote that these three new axes are not all aligned alongthe crystal axes, it is convenient to choose axis 3 to be parallel to the direction along whichthe condition of plane strain is invoked, so that 33 = 0, and to choose 1 to be the directionalong which a stress is applied, with the stress 22 along 2
set to zero. Hence, we have theequations
11 = S 1111 11 + S 1133 33,33 = S 3311 11 + S 3333 33 = 0.
Using the second of these equations to substitute for 33 in the first of these equations, it isapparent that the plane strain Youngs modulus E parallel to the direction 1 is defined bythe expression
E = 11
S 1111S3333 S 1133S 3311
Using the contracted two suffix Voigt notation for the Sijkl (see the Appendix), this equationsimplifies to the form
E = s33
s 11s33 s 213
Equation (5) can be written in an equivalent form:
E = (1/s11)
Now, 1/s 11 is Youngs modulus E along the direction 1 , while the ratios s 13/s 11 and
s 31/s 33 both define Poisson ratios. Using the nomenclature used by Norris  we candefine 13 to be the ratio s 13/s 11, corresponding to the ratio of the negative strain along
150 K.M. Knowles
3 to the positive strain along 1 when a tensile stress is applied along 1; similarly we candefine 31 to be the ratio s 31/s 33. Hence, dropping the primes for convenience, Eq. (6) canalso be rewritten conveniently in the form
E1 = E1(1 1331) , (7)
where the 1 subscripts on E and E indicate the direction along which the stress is applied.It is evident that this equation is similar to, but not the same as, the form of the equationquoted by Hopcroft et al.  for what they termed the plate modulus in their Eq. (11)when considering the elastic deflection of short, relatively wide beams of single crystals.
For a general anisotropic material with known elastic constants, numerical manipulationof Eq. (5) enables the plane strain Youngs modulus to be computed for general choices ofcrystallographic directions 1 and 3. Fortunately, for cubic materials such as silicon, thereare only three ind